What is RT?
The term Rapid Tooling (RT)
is typically used to describe a
process which either uses a
Rapid Prototyping (RP)
model as a pattern to create a
mould quickly or uses the
Rapid Prototyping process
directly to fabricate a tool for
a limited volume of
What is RT?
• Making tools using RP process to
Minimize the cost
Increase the productivity
Increase dimensional accuracy
Decrease total time
How is it different from conventional
• Tooling time is much shorter than for a
conventional tool. (almost below one-fifth
that of conventional tooling)
• Tooling cost is much less than for a
conventional tool. (Cost can be below five
percent of conventional tooling cost).
• Tool life is considerably less than for a
• Tolerances are wider than for a
Types of RT
Rapid Tooling can be broadly classified as:
1. Indirect Tooling
2. Direct Tooling
• Indirect tooling methods used RP inserts to
• But direct RT methods allow injection moulding
and die-casting inserts to build directly from 3D
• Indirect or Pattern-based Tooling
approaches use master patterns to
produce a mould or die, and Direct
Tooling, where the additive process
builds the actual moulds.
Indirect Tooling (Pattern Based
• Indirect tooling methods are intended as
prototyping or pre-production tooling
processes and not production methods.
• Most any rapid prototyping process can
yield patterns for indirect tooling.
Techniques for Indirect RT
1) RSP Tooling
2) Reconfigurable Tooling
3) Silicone Rubber Tooling
4) Aluminum filled Epoxy Tooling
5) Spray Metal Tooling
6) Cast kirksite
7) 3D Keltool
Silicone Rubber Tooling
• One of the most popular tooling applications
for RP is the production of room temperature
vulcanizing (RTV) silicone rubber tooling
• The purpose of RTV tools is to create
urethane or epoxy prototypes, often under
vacuum (hence the term vacuum casting)
The process of making a rubber mould consists of:
• Making a master pattern, usually on an RP machine.
• Finishing the pattern to the desired appearance.
• Casting RTV silicone rubber around the pattern to
form the mould, and then injecting the mould with
two-part thermoset materials to create moulded
• Silicone rubber tooling provides fast, inexpensive moulds,
excellent part cosmetics, and the option of using multiple
• The process is suitable for small or medium-sized parts
• Another benefit of silicone rubber tooling is the negative
draft (undercuts) that can be achieved due to the flexibility
of the mould material
Aluminium filled epoxy tooling
• Its also known as ‘Composite
• Like silicone rubber tooling,
epoxy-based composite tooling
requires a master pattern
• This pattern is created by RP
• The pattern is finished and then
embedded in a parting line block
to create the parting line of the
• Metal inserts are placed in areas where the epoxy is
unlikely to withstand the pressures of the injection-
• Epoxy is then cast against the pattern and parting line
block combination to create the first side of the tool.
• Once the epoxy has cured, the assembly is inverted, and the
parting line is removed, leaving the pattern embedded in
the first side of the tool.
• The second side of the tool is then cast against the first.
• Composite tooling generates injection moulded parts in 2 to 6 weeks
• The moulding process will have a cycle time of 5 to 15 minutes
• Accuracy is dependent on the SLA model. Typically about +/-0.005" to +/-
• Dependent upon the cost of the master pattern, and overall size of the part.
An SLA master pattern can cost between $300 to $1000, on average, and the
epoxy tool is typically between $800 and $1000
Spray metal tooling
• It is very similar to aluminum filled epoxy
• In this process, against the RP pattern low temperature
metal alloys is sprayed
• A thin metal coating is then arc-sprayed on the resultant
• It gives higher strength and maximum tool life
• This process is suitable for larger parts
• Very good for large parts
• No or less shrinkage
• Highly accurate
• RSP stands for Rapid Solidification Process
• We create a plastic model using SLA
• And then we make moulds with either by epoxy tooling or spray
metal onto it
• But most of the cases, ceramics are used
• What’s significant in that is that we atomize the metal down to as
small as 5 microns.
• When the metal hits the ceramic, because of the small size of the
droplets, they freeze very quickly, thus the rapid solidification.
• This process results in extremely fine grain structure and the
alloys generally stay in solution and there is very little internal
• Kirksite is a zinc-aluminum alloy with excellent
wear resistance. (94 percent Zn, 6 percent Al) with a
melting point of 385oC)
• The process for making cast kirksite tooling begins
much like the process for epoxy-based composite
tooling, except that two additional reversals are
required to permit the creation of tooling in a more
Cast Kirksite Process:
• First, a shrink-compensated master pattern of the part is
produced, typically using an RP process.
• A rubber or urethane material is then cast against the part
master to create patterns for the core and cavity set, which
will be cast in kirksite.
• Plaster is then cast against the core and cavity patterns to
create moulds into which the kirksite is cast.
• Once the kirksite is cast into the plaster moulds, the plaster
is broken away, and the kirksite core and cavity are fit into
a mould base
• 3D Keltool is a powder metal process used to make
injection-mould inserts and other durable tooling from
• It is very similar spray metal tooling
• Keltool was originally developed by 3M in 1976 and
was sold and further developed by Keltool Inc. In 1996,
3D Systems purchased the technology from Keltool
Inc. and renamed it 3D Keltool
• The word "Keltool" refers to the proprietary powder metal
sintering process, which involves infiltrating a fused
metal part with copper alloy.
• This alloy fills in the voids in the otherwise porous
material, producing a surface with the finish and
hardness necessary for an injection mould
Process chain of 3D Keltool:
I. Master pattern
II. Silicone casting
III. Casting with a tool steel/Tungsten carbide/epoxy mixture
IV. Burn-out of binder, sintering and infiltration with copper in
V. Tool insert ready for production
• This process requires a master pattern, typically an SLA
model, that can be used to develop a silicone mould
that will then be used to produce the Keltool mould.
• The Keltool mould is then processed with a copper
infiltration and sintered to increase its strength and
cure the mould.
• The finished Keltool part has the hardness of a A6 Tool
Steel and can be machined like a traditional hard tool.
• Very similar to injection moulding
• But here we use thermosetting polymers
• RIM requires a curing reaction to occur within the
RIM (Reaction Injection Moulding)
• Two highly reactive
together in a
injected into a
heated mold under
• The mixture is
allowed to sit in the
mould long enough
for it to expand and
Common items made via RIM
include automotive bumpers, air
spoilers, and fenders (used for mud
Direct AIM (ACES Injection Moulding)
• In the AIM process, the mould is "grown" using the SLA
• The mould is similar to a regular part SLA, but is the
negative image and cut into two halves.
• The cavity can be filled with a variety of materials,
• Aluminum-filled epoxy
• Low-melt temperature metals
• QuickCast is a process that allows for the creation of
direct shell investment castings using "QuickCast"
Stereolithography (SLA) patterns.
• The QuickCast method allows you to rapidly build
highly accurate resin patterns in Stereolithography,
bypassing the expensive and time-consuming step of
• QuickCast facilitates rapid production of small
quantities of metal parts in much less time than
• Instead of the SLA part being completely solid,
QuickCast eliminates 95% of the internal mass of the
• This process uses the essence of SLS
• Here we use Copper Polyamide powder matrix
• Copper Polyamide is a new metal plastic composite
designed for short tooling applications
• Tooling inserts are produced directly in the SLS
machine with a layer thickness of 75 µm.
• Subsequent finishing is necessary before their
integration in the tool base.
• During the CAD stage, Copper polyamide inserts a
shelled and cooling lines, ejector pin guides, gates and
runners are included in the design and built directly
during the SLS process.
• Then the insert surface are sealed with epoxy
and finished with sand paper and finally the
shell inserts are packed up with a metal alloy.
• Inserts produced from copper polyamide are easy
to machine and finish.
• Heat resistant and thermal conductivity are better
in most plastic tooling materials.
• The cycle times of moulds employing copper
polyamide inserts are similar to those of metal
Powder feed position
Metal powder bed
• Currently available alloys used in the process
include 17-4 and 15-5 stainless steel, maraging steel,
cobalt chromium, inconel 625 and 718, and titanium
• Theoretically, almost any alloy metal can be used in
this process once fully developed and validated.
• DMLS is a very cost and time effective
• DMLS is used to manufacture direct parts for a
variety of industries including aerospace, dental,
medical and other industries that have small to
medium size, highly complex parts and the tooling
industry to make direct tooling inserts.